The atomic force microscope (AFM) has very much improved our capabilities to image, probe, and manipulate objects on surfaces, especially for soft and polymeric materials. Among all the different developments, which include single molecule imaging [158, 179, 180], measurements of forces and friction [170,
176, 181, 182], the possibility to probe and manipulate single macromolecules seems most exciting [27, 50, 51, 149, 164, 183, 184].
Among these developments, the so-called single molecule force spectroscopy became a widely used tool to investigate the mechanical properties of single macromolecules and their interaction with surfaces
[23, 27, 28, 47, 51, 162, 183, 185, 186]. The technique relies on a configuration where the substrate and the tip are bridged with a single polymer molecule, and one analyzes the measured force-distance curves, normally upon retraction, but eventually also upon approach. Two main classes of events can be normally observed, namely pulling and peeling events. A pulling event resembles a spike in the force curve, and ideally corresponds to the force-extension relationship of a single polymer molecule, which is firmly attached to the substrate and to the tip [28, 35, 49, 51, 150, 170]. Such force profiles can be interpreted by the freely jointed and worm-like chain models including chain elasticity. A peeling event is characterized with a plateau in the force curve, which reflects the force that is necessary to peel off the adsorbed molecule, or eventually to slide it along the substrate [8, 14, 37, 153, 187-189]. These forces reflect the affinity of the molecules for the surface, and can be related to the type of substrate and its charge. These events also may occur in succession. A series of spikes resembling the tooth of a saw is normally interpreted as the unwrapping of individual macromolecule domains, which are frequently observed for muscle proteins (e.g., titin, tenascin) [26, 27]. A series of peeling events, which resemble a staircase, are typically due to the peeling of several molecules from the surface, even though they could also be caused by a combination of sliding and peeling [8, 39, 153, 190]. Frequently, however, many of these events occur in combination, and the respective force profiles have complex, random appearances, which are difficult to interpret. The present focus of this chapter is the identification of the methodology to obtain the single-molecule stretching response from pulling events.
Figure 4.1 Probing the force response of single polymer molecules with the AFM. (a) Methods used to pick up single polymer molecules. Nano-handling involves a single adsorbed polymer identified by imaging. Classical pulling lifts single molecules from an adsorbed polymer layer. Fishing uses polymers adsorbed to an AFM tip. (b) Available techniques to stretch single polymer molecules. The no clamping technique pulls molecules from contact to large distances resulting in their complete detachment. The contact clamping technique repeatedly stretches and relaxes an attached polymer molecule to its maximal extension but contacts the surface in between. The non-contact clamping technique also stretches and relaxes a polymer but avoids contacting the surface in between. (c) Identification of single molecule events by force normalization. Recording stretching events versus distance x and identification of distances xicorresponding to the reference force F0(left) and superposition of the force profiles versus normalized extension x x/ i (right).
To generate a single bridging polymer molecule between the substrate and the tip, various methods have been proposed, see Figure 4.1a. The nano-handling method identifies a single adsorbed polymer molecule on the surface by AFM imaging, and this molecule is probed with the AFM tip through repeated approach-retraction cycles [37, 51, 191]. A bridging event is localized by its force response. The configuration of the adsorbed molecule can be again probed by imaging after the force experiment. The classical pulling method is by far the simplest to realize and therefore the most popular [28, 170]. This method relies on a substrate with an adsorbed polymeric layer, and this substrate is probed with repeated approach-retraction cycles. A bridging event is identified by spikes or plateaus in the force curve. The fishing method is similar, but the polymers are adsorbed to the AFM tip [137, 188, 189, 192]
. Whether the polymers will be picked up in a given configuration, and whether they will be stretched or peeled, depends strongly on the solution conditions, the nature of the substrate and the tip, and their surface functionalization. When the affinity of the polymer to the substrate is strong, no events will be observed, while when this affinity is weak, peeling events will be observed. Pulling events normally occur when the affinity is intermediate.
Once a molecule has been picked up, the retraction part of the force curve reveals whether it is being peeled or pulled. The mechanical response of individual polymer molecules can be only extracted from pulling events. Such response can be obtained in different ways, see Figure 4.1b. The no-clamping technique relies on approach-retraction cycles that start at larger separation distances and go through the contact region [28, 170]. In this mode, each bridging polymer detaches from the tip after each retraction. The contact clamping technique permits to access the reversibility of the stretching force response of an individual polymer [35, 47, 65, 150].Within this technique, one retracts the tip from the surface only to the point that the polymer is being stretched, but without detaching it. Hysteresis of the force curves upon approach and retraction indicates slow conformational transitions or refolding domains [52, 166, 167]. The cycle is completed by approaching the tip again into contact. With this technique one cannot ascertain, whether the same or a different polymer molecule is being extended within subsequent cycles. The non-contact clamping technique avoids this problem, since the tip is not approached to contact, whereby one avoids the possibility that the polymer chain is being exchanged. Techniques involving combination of lateral and normal displacement of the tip were equally proposed, but they will not be pursued here further.[8, 39]
Whether an observed pulling event originates from the stretching of a single or several polymer molecules is not necessarily obvious. Several tests were proposed that can be used to identify such events.
(1) When one uses the no-clamping technique, several pulling events may occur in succession upon retraction of the tip. Obviously, the last event likely corresponds to a single molecule. (2) Models of force-extension relationships suggest that the force-extension relationship is only a function of the extension relative to the contour length. Therefore, the force profiles corresponding to single molecules
will collapse upon a master curve when plotted versus the normalized extension that corresponds to a given force, see Figure 4.1c. (3) Performing fishing instead of classical pulling experiments will increase the probability to pick up a single molecule since the polymers are adsorbed on the tip only. (4) The force response of a single polymer ought to be reversible, and therefore the profiles obtained from approach and retraction curves should superpose. However, this test requires clamping of the molecule, which is experimentally not always feasible. (5) Most straightforward is to identify a single adsorbed polymer by imaging, and obviously, force extension experiments carried out in this configuration necessary involve single molecules only.
The aim of the present chapter is to demonstrate that not all these tests to identify single molecule stretching events are reliable. In particular, only the (4) reversibility and (5) single molecule seem reliable. On the other hand, the different tests including (1) last event, (2) master curve, and (3) fishing experiments, may prove unreliable and should be used with caution. We shall illustrate these facts with pulling experiments carried out with amino-functionalized dendronized polymers of generation 1 and 3, which are abbreviated as PG1 and PG3. Their structures are summarized in Figure 4.2.
Figure 4.2 Structural formulas of the polymer used in this study. Amino-functionalized dendronized polymers of generation 1 and 3, abbreviated as PG1 and PG3. Polymers are positively charged at the conditions investigated.
4.2 Experimental section
Polymers. Polymethacrylate-based dendronized polymers (DPs) of different generations, 1 and 3, denoted as PG1 and PG3, terminated with amine groups were synthesized with the attach-to route as described previously [80, 154]. The polydispersity index of the side dendrons is about 1.01 with respect to
the expected number of the amine groups for each repeat unit. The characterization of these DPs by gel permeation chromatography and AFM is discussed elsewhere [37, 80, 154]. DPs were dissolved in electrolyte solutions adjusted to pH 4.0 with HCl, and the ionic strength was eventually adjusted with KCl. Under these conditions, the amine groups are positively charged.
Substrates. The experiments were carried out with bare mica, functionalized mica, and functionalized silica. Mica surfaces were obtained by cleaving high-grade mica (Plano Wetzlar, Germany) with adhesive tape. Amino-functionalized (AF) mica was obtained by placing the freshly cleaved mica sheet in an evacuated glass container aside a 30 µL drop of 3-(ethoxydimethylsilyl)propylamine (Sigma Aldrich, Switzerland) for 12 h. Epoxy-functionalized (EF) silica was prepared with naturally oxidized silicon wafers from Silchem (Canada). The wafers were cleaned for 20 min with Piranha solution, which consists of a mixture of H2SO4 98% and H2O2 30% in a volumetric ratio of 3:1. The wafers were washed with Milli-Q water, dried in a stream of nitrogen, and placed in an evacuated container aside a 150 µL drop of (3‐glycidoxypropyl)dimethylethoxy-silane (Sigma Aldrich, Switzerland) for 2 h.
High-resolution AFM imaging. Imaging in air was performed with a Cypher (Asylum Research, Santa Barbara, CA). This instrument was also used to carry out all subsequent AFM experiments. High-resolution images were acquired in amplitude modulation mode with super sharp silicon tips (SSS-NCHR, Nanosensors, Neuchatel, Switzerland). These cantilevers have a nominal tip radius below 5 nm, a resonance frequency in air around 330 Hz and spring constant of 42 N/m. Images were acquired in air near the resonance frequency of the cantilevers with a speed of 300 nm/s. The free oscillation amplitude (FOA) was adjusted to around 15 nm.
Nano-handling. Biolever mini cantilevers with silicon nitride tips (BL-AC40TS, Olympus, Japan) were used. These tips have a nominal tip radius below 10 nm and resonance frequencies around 30 kHz in water and around 130 kHz in air. The spring constants were in the range of 0.07–0.15 N/m as determined in air by the thermal fluctuation method. The cantilevers were cleaned in a UV-ozone cleaner (PSD Pro, Novascan, Ames, USA) for 20 min in an oxygen-enriched atmosphere and epoxy-silanized overnight with (3-glycidoxypropyl)-dimethylethoxysilane as described above. The substrates used for the experiments were AF-mica or EF-silica. The substrates were incubated in polymer solutions at concentrations of 4–6 mg/L for 40 s. A sufficient coverage of DPs on the surface was obtained at this concentration, but minimizing the overlap of different chains. Subsequently the sample was rinsed with water and dried with a stream of nitrogen. The substrates were again incubated in the respective electrolyte solution, and images were acquired in solution. No effect of intermediate drying of the sample on the experimental results was observed, as verified in selected experiments by keeping the sample in wet state. However, the
procedure involving the intermediate drying was more practical during the sample preparation and the mounting of the sample in the AFM cell. Thereby, the scan rate was set to 4.9 Hz, FOA about 20 nm, and a set point corresponding to around 70% of the FOA. After stabilization of the image, the piezo excitation of the cantilever was stopped, and the tip was positioned over the end of a selected polymer. Vertical approach-retraction cycles through the contact region were then recorded with a sampling rate of 2 kHz, approach-retraction velocity of 200 nm/s and a maximum deflection set point towards the surface of 30 nm. The initial pull-off distance was chosen to be about one quarter of the molecular length, which was read from the image. Once a molecule is picked up, the pull-off distance is initially increased to obtaine larger forces and extensions, which are then kept to record a larger number of force curves. This process is continued until the molecule falls off, which normally happens after 2–10 cycles. This protocol corresponds to the contact clamping mode (Figure 4.1b). The piezo displacement and cantilever deflection were converted to force-distance curves, resulting in a noise in the force curves of about 0.01 nN. After the force measurements, the same region was imaged again in order to observe the displacement of the targeted molecule. More details on such nano-handling experiments can be found elsewhere .
Classical pulling and fishing experiments. For the classical pulling experiments the substrates were coated with polymers. Thereby, the respective substrates were incubated in the appropriate polymer solution with a concentration of 80 mg/L for 40 min, rinsed with pure electrolyte solution, then with pure water, and dried. The biolever mini cantilevers were epoxy-functionalized as described above. For the fishing experiments, the functionalized cantilevers were incubated in the respective polymer solutions in the same way. The excess solution was removed with an absorbing tissue, and dried. The AFM cell was assembled with the respective substrate, filled with the appropriate electrolyte solution, and the pulling experiments were carried out with repeated approach-retraction cycles with a sampling rate of 2 kHz. The other parameters are the same as given above. The experiments were carried in different modes. Either the cycles were run through the contact region out to larger pull-off distances of more than 200 nm. This procedure is the no-clamping mode (Figure 4.1b). Whenever possible, the molecules were clamped. In this case, the cycles were run through the contact region and the pull-off distances were initially chosen to be only 20–40 nm. Once a molecule was picked up, the distance was further increased until larger forces and extensions were obtained. At this maximum distance, the forces curves were recorded during several cycles, until the molecule would fall off. At that point, the pull-off distance is decreased again until another molecule is picked up. This protocol is the contact clamping mode (Figure 4.1b). The non-contact clamping mode is carried out in the same way, except once the molecule is pulled to the maximum distance, the cantilever is only partially re-approached to the surface, typically 30–50% of the maximum
distance, but not closer than about 20 nm to the surface. Within these conditions, several cycles are recorded.
4.3 Results and discussion
This study compares the stretching force response of individual adsorbed dendronized polymers with the same polymers picked up from dense adsorbed layers. First, we discuss results obtained with the nano-handling technique, as it allows studying the response of a single polymer. Subsequently, these results are compared with the classical pulling technique, where the polymer is being picked up from dense layer adsorbed on a flat substrate. Finally, we use the fishing technique, where the molecules are adsorbed to the AFM tip. In some situations, the molecules were clamped and multiple force extension curves were recorded with the same molecule, either contacting the substrate in every cycle or not. In these cases, we refer to contact or non-contact clamping, see Figure 4.1b. Most experiments were carried out with PG3, but some comparison experiments were equally carried out with PG1. Two ionic strengths were compared, namely 0.1 mM and 100 mM.
Figure 4.3 Single-molecule nano-handling force experiment with PG3 adsorbed on EF-silica in 0.1 mM electrolyte solution at pH 4. Adsorbed polymer is imaged before (a) and after (b) the force measurements. The arrow indicates the position on the molecule where the force experiment is performed. (c) The molecule is picked up by the functionalized AFM tip and a series of approach and redraw force curves are recorded. (d) Force-extension profiles from both approach and redraw part of the force curves are plotted versus normalized extension.
Nano-handling with PG3. The force response of single polymer can be best studied with the nano-handling technique. PG3 was adsorbed from a dilute aqueous solution of low ionic strength of 0.1 mM to
an EF-silica substrate. An AFM image of the adsorbed molecules is shown in Figure 4.3a. The tip is then positioned over a selected end of a polymer molecule (arrow) and a series of vertical approach and retraction force profiles is recorded. The tip is only retracted to about 30 nm. During the first approach (1) the polymer is not being picked up, as can be seen from the featureless retraction curve at larger distances.
The second approach (2) was successful, as the retraction curve shows that the polymer is being lifted from the surface. The following approach profile (3) shows the elastic response of the polymer. Note that the largest distance shown in retraction curve shown in (2) corresponds to the largest distance shown in the approach curve (3). The minor difference is caused by drift. The polymer is now lifted up again, but as shown in the retraction curve (3), it is once again pulled further out. The elastic response during approach is shown in (4). By repeating these experiments, as in traces (5) and (6), the polymer is lifted up further away from the surface, and a longer stretching response can be recorded. Under these conditions, the polymer interacts only weakly with the surface, such that also the approach curve yields clean force extension curves. At one point, the polymer detaches (7). After detachment, the same region is imaged again. One observes that the polymer is again adsorbed at the same location, probably due to the existence of some preferential adsorption sites. In this way, force curves can be recorded with the same polymer upon approach and retraction. When one uses the first cycles to lift the polymer further away from the surface, one often obtains force extension curves that cover a larger force range. On the other hand, when one pulls too far, one risks detaching of the polymer that was picked up. With the contact clamping, the technique (Figure 4.1b) works well, and by selecting several polymers on the surface, a large number of force profiles extending over a wide force range can be obtained. The force F x( ) that is measured as a function of the distance x is normalized by determining the distance xi that satisfies F x( )i F0 where F0 is an appropriately threshold force (see Figure 4.1c). The forces are then plotted versus the normalized extension x x/ i in Figure 4.3d. The threshold force is chosen to be F00.25 nN. One observes that the forces profiles recorded upon approach and retraction collapse upon a common master curve, confirming that the extension process is fully reversible.
A similar experiment carried out at a high ionic strength of 100 mM is shown in Figure 4.4. The EF-silica cannot be used as a substrate since the molecules adhere too strongly to the surface under these solution conditions, and the molecules cannot be picked up. However, sufficient number of stretching events can be obtained with AF-mica. Nevertheless, the molecules are often interacting strongly with the substrate upon retraction, evidenced by the various desorption steps and saw tooth-like pattern in the retraction part of the force curve. Therefore, no force extension profiles can be obtained upon retraction.
On the other hand, approach curves provide the force profiles. The respective force extension profiles
were again normalized to 0.25 nN, and they are shown in Figure 4.4d. Comparison of the image before and after the experiment shows that the molecule has been slightly displaced during the force experiment.
Seemingly, there are some preferential adsorption sites, which cause the molecule to readsorb in a very similar conformation. In the example shown in Figure 4.3, the change in the polymer conformation before
Seemingly, there are some preferential adsorption sites, which cause the molecule to readsorb in a very similar conformation. In the example shown in Figure 4.3, the change in the polymer conformation before